FLEXURE OF STRUCTURAL
Please return to:
Wood Engineering Research
Forest Products Laboratory
Madison, Wisconsin 53705
UNITED STATES DEPARTMENT OF AGRICULTURE
FOREST PRODUCTS LABORATORY
In Cooperation with the University of Wisconsin
FLEXURE OF STRUCTURAL SANDWICH CONSTRUCTION
EDWARD W. KUENZI, Engineer
Forest Products Laboratory,? Forest Service
U. S. Department of Agriculture
This paper presents some of the basic theories of flexure, particularly as
applied to sandwich constructions. Consideration of various methods of applying
loads and a theoretical analysis of a particular type of loading resulted in
the conclusion that measurenents of stiffness and strength may best be obtained
by testing under two-point loading, preferably at two quarter-span points. A
formula is presented for de.:.ermining the approximate span, so that shear deflec-
tions can be easily measured. Flexural strength, the nonelastic flexure of
sandwich construction, and the clamping of sandwich constructions are discussed
Flexure testing of a material was perhaps one of the earliest means of evalua-
ting stiffness and strength. Observations on the bending behavior of different
woods probably aided primitive man in selecting the proper stone-ax handle or
bow and arrow. This type of "hand" testing is usually conducted by anyone who
is handed a piece of material to inspect. The tester advances comments con-
cerning the material's amazing stiffness and strength, if appropriate, or per-
haps a comment as to how poorly the material behaves. Uses for the material are
often suggested if it appears to be unusually stiff and strong, or, if the
material is weak, it may be hinted that there is no possible application.
The result of the "hand" . testing must be properly interpreted. The ultimate use
of the material and the performance requirements-ofthe finished product must
be carefully considered. A string or wire will fail to meet the lowest flexure
requirements, but both find wide use as tensile structural elements. Often the
–Presented at a meeting of American Society for Testing Materials Committee
C-19, on structural sandwich construction, in Washington, D. C. October
?Maintained at Madison, Wis., in cooperation with the University of Wisconsin.
Rept. No. 1829 -1- Agriculture-Madison
shape of the finished product contributes more to successful performance than
the material itself. For example, thin, flexible sheets of steel are now being
used for more or less acceptable automobile bodies.
The invention of testing machines has provided means for obtaining more
quantitative information concerning materials than can be obtained by "hand"
testing. These machines and all of their modern, automatic gadgets, however,
must be used with caution in order to arrive at sensible conclusions concern-
ing the behavior of a material.
Possibly, the salient question to be considered before performing a test is
"What is to be evaluated?" It certainly would not be helpful to determine the
tensile strength of concrete that is to be used in compression. It may be
feasible, however, to conduct quality-control tests in tension rather than in
Compression. Similarly, for most materials, it is not necessary to conduct
flexure tests in determining mechanical properties, although it may be feasible
to conduct quality-control tests in flexure. Flexure tests may be, in fact,
exactly what is needed to evaluatd the adequacy of constructions.
Testing, therefore, is somewhat divided into two parts, quality-control tests
and evaluation of mechanical properties. The principal concern of this paper
is the evaluation of mechanical properties.
The Flexure Test
By means of the flexure test, loads can be applied to the test specimen to
produce_censtant or variable bending moments and constant or variable shears.
Conditioas at the'reactions can be clamped or simply supported. The actual
type of loading and support should be considered in view of what information
is to be obtained.
Uniformly distributed loads can be experimentally applied by various ways, but
these are usually costly and time-consuming.
Clamping of the ends of a beam or the edge of a panel is never accomplished
successfully by empirical means. It can be shown, however, that the effective
experimental clamping can be empirically determined for use in calculating
maximum bending moments and shears.
The method remaining is the use of concentrated loads to produce. constant shears
and constant or variable bending moments in a specimen' simply supported at the
The simplest load to apply is a single, concentrated load applied at midspan.
This center loading produces stress concentrations at the load point of twice
the magnitude of corresponding stress concentrations at the reactions. The
point of maximum moment is at the load point, Thus, if the material is not
homogeneous, a weak spot near the reactions would not be discovered by testing
under a single load., In sandWich constructions particularly, the stress at
which a facing wrinkle appears is mostly a guess, because the facing is held to
the core at the point of maximum moment.
Rept. No. 1829 -2-
The load may also be applied through two points, preferably symmetrically
placed with reference to the midspan point for simplicity. The use of two-
point loading produces constant bending moments in the portion of the specimen
between the loads and constant shears in the portions outside the loads. Thus,
within the central section, more of the material is stressed to the same amount
in two-point loading than in center loading, and failure due to moments will
begin at the weakest point. Stress concentrations still exist at the load
points, but they are one-half the magnitude of those applied with a single load
and are equal to concentrations at the reactions.
How are the load points to be spaced? The ultimate use of many constructions
is to withstand uniformly distributed loads. If the loads are applied at two
quarter-span points, the greatest moments and shears produced will-be equal to
those applied by uniformly distributed loads. Therefore, the best method, of
loading in a flexure test is to apply two concentrated loads at the quarter-
span points on a beam simply supported at the reactions.
From the test data of a beam, the stiffness and strength will undoubtedly be
computed. For most materials, the beam deflection depends mainly upon the
modulus of elasticity of the material. There is always some additional deflec-
tion due to shear, but this is usually so small that it is neglected. For
sandwich constructions, however, the core material has a relatively low shear
modulus, and the beam may deflect a considerable amount because of shear defor-
mations. This low shear modulus of the core will also decrease the buckling
loads of plates and shells. Since neglect of proper consideration of the shear
modulus of the core may lead to unconservative prediction of deflections or
critical loads, it is essential that the modulus be determined in order that its
effect may be taken into account.
One way to determine the shear modulus of a core of structural sandwich construc-
tion is by means of a flexure test under two-point loading. The two-point
loading allows the central portion of the beam to bend under constant moment
without shear, and, therefore, the stiffness of the sandwich construction with
no shear deflection may also be obtained by proper measurement of deflections.
The span of the test specimen should be chosen so that deflections due to shear
are sizeable as compared to bending deflections. The following discussion and
derivation give the formulas for analyzing the test data for a sandwich beam
simply supported at the reactions and loaded at two quarter-span points
The beam is assumed to be loaded with a total load, P, equally applied at two
quarter-span points, each spaced a distance, , from the reactions on a total
The general expression for the curvature of a beam, assuming positive deflections
downward and the axis origin at the left reaction (x positive to the right), is
3---Timoshenko, S. Strength of Materials, Part I. New York. 1940.
Rept. No. 1829 -3-
2 M Vsu = x 4. x)
where y = deflection (measured positive downward)
x = distance from left reaction
M = bending moment (positive bending produces, positive curvature)X
D = bending stiffness of beam
Vx = shear load (shear is positive if the force on the positive side
an elemental beam length is in the positive z direction)
N = shear rigidity of beam
The deflection is determined by solving formula (1). As usual, the beam is
considered in its several parts:
Section 1, from x = 0 to x—= a/4,
Mxl = 2 7x1 =
thenand 2y) = Px 1 (dVx)
2D N dx
Px3 + C ix + C2
Y1 = - 12D 2n
When x = 0, y = 0. Therefore, C 2 = 0
Y1 = 12D clx
Section 2, from x = a/4 to x = 3a/4,
M = Pa Vx2 . 0x2 87-
(d2y, \, _ Pa
6-.2( ) 2
- Pax + c3
Sept. No. 1829 -h -
When x = a/2, tif = 0. Therefore, Pa2
Paxand dy +
dx / 2 toD loD